*HERON Vol. 57 (2012) No. 2 *

**Using particle packing technology for ** **sustainable concrete mixture design **

Sonja A.A.M. Fennis, Joost C. Walraven

Delft University of Technology, the Netherlands

**The annual production of Portland cement, estimated at 3.4 billion tons in 2011, is responsible **
**for about 7% of the total worldwide CO****2****-emission. To reduce this environmental impact it is **
**important to use innovative technologies for the design of concrete structures and mixtures. **

**In this paper, it is shown how particle packing technology can be used to reduce the amount **
**of cement in concrete by concrete mixture optimization, resulting in more sustainable **
**concrete. First, three different methods to determine the particle distribution of a mixture are **
**presented; optimization curves, particle packing models and discrete element modelling. The **
**advantage of using analytical particle packing models is presented based on relations **
**between packing density, water demand and strength. Experiments on ecological concrete **
**demonstrate how effective particle packing technology can be used to reduce the cement **
**content in concrete. Three concrete mixtures with low cement content were developed and the **
**compressive strength, tensile strength, modulus of elasticity, shrinkage, creep and electrical **
**resistance was determined. By using particle packing technology in concrete mixture **

**optimization, it is possible to design concrete in which the cement content is reduced by more **
**than 50% and the CO****2****-emission of concrete is reduced by 25%. **

**Key words: Aggregate, cement spacing, concrete, flowability, particle packing, optimization **

**1 ** **Introduction **

Nowadays, sustainability is one of the main focuses of attention in concrete industry.

Though concrete is a structural material of which the total environmental impact per cubic meter is limited, compared to similar types of building materials, the CO2-emission resulting from cement production is large, because of the vast amount of cement and concrete produced yearly. To produce Portland cement, calcination of limestone is required and during this chemical process about 0.5 kg CO2 per kg of cement is released,

not yet taking into account the CO2-emission from the fuel burning required for this process. The annual production of Portland cement, estimated at 3.4 billion tons in 2011 [minerals.usgs.gov], is responsible for about 7% of the total worldwide CO2-emission [Mehta, 2001; ecosmartconcrete.com; pbl.nl]. Taking environmental measures would be good, especially when it is realised the worldwide production of Portland cement has doubled over the past 10 years from an estimated 1.7 billion tons in 2001 to 3.4 billion ton in 2011 [minerals.usgs.gov]. Replacing concrete by other building materials would not solve this environmental issue. Therefore, the solution should be found in reducing the environmental impact of concrete itself. In some applications, where strength of concrete is governing, this can be achieved by using a stronger type of concrete so less material is required [Gorkum, 2010]. For other applications, where strength is not the governing design criterion, concrete mixtures that contain less cement can be used. In all cases it is important to design concrete structures and mixtures in such way that the environmental impact is minimized. Therefore, in the literature review part of this paper it is presented in which ways particle packing technology can be used to support concrete mixture

optimization. Furthermore, the paper shows that particle packing can be used to increase the strength of concrete while reducing the amount of cement, leading to considerable CO2

reduction.

**2 ** **Particle optimization methods: a literature review **

Particle packing optimization in concrete mixture design covers the selection of the right
sizes and amounts of various particles. The particles should be selected to fill up the voids
between large particles with smaller particles and so on, in order to increase the particle
packing density α*t*. The definition of particle packing density α*t* is the solid volume of
particles in a unit volume. In the history of concrete, the concept of packing of aggregates
already received interest in the 19^{th} century [Féret, 1892], but especially the last decades,
particle size optimization has gained new interest with the introduction of new types of
concrete, such as high performance concrete, self-compacting concrete, fiber reinforced
concrete and ecological concrete. Particle optimization methods can be divided into three
groups:

• *Optimization curves. Groups of particles, with a specific particle size distribution, *
are combined in such a way that the total particle size distribution of the mixture
is closest to an optimum curve. (Subsection 2.1)

• *Particle packing models. These models are analytical models that calculate the *
overall packing density of a mixture based on the geometry of the combined
particle groups. (Subsection 2.2)

• *Discrete element models. With numerical models a ‘virtual’ particle structure from a *
given particle size distribution is generated. (Subsection 2.3)

**2.1 Optimization curves **

After Féret stated in 1892 that the choice of aggregates influences concrete strength [Féret,
1892], many researchers tried to find the ideal grading curve. In this area the most well-
known researcher is Fuller with his famous Fuller curve [Fuller and Thompson, 1907]. Mix
design calculations based on his curve are still used today. The Fuller curve is described by
Equation 1 with *q*= 0.5 [Talbot and Richart, 1923]. See also Figure 1. The curve should
represented the grading with the greatest density, based on their conclusions that the
gradation that gives the greatest density of the aggregates alone may not necessarily give
the greatest density when combined with water and cement because of the way the cement
particles fit into smaller pores.

Some researchers tried to improve this curve, like [Andreasen and Andersen, 1930].

They proposed the use of an exponent *q*in the range of 0.33 – 0.50. This adjustment factor
*q*had to be determined experimentally and therefore can differ depending on the
characteristics of the particles. With angular coarse particles the ideal curve would be best
prescribed with a lower value for*q*, since more fine particles should be added to fill the
voids between the coarse particles [Kumar and Santhanam, 2003].

max

( )
*d* *q*

*P d* *d*

=

^{ (1) }

( )

*P d* size cumulative distribution function [-]

*d* particle diameter being considered [m]

*d*max maximum particle diameter in the mixture [m]

*q* parameter (0.33-0.5) which adjusts the curve for fineness
or coarseness [-]

In 1980 Funk and Dinger recognized that any real size distribution must have a finite lower
size limit *d*_{min}[Funk and Dinger, 1980]. So, in contrast to the Fuller curve their ideal size
distribution not only pays attention to the largest grain but also to the smallest used grain.

*Figure 1: Ideal packing curves according to Fuller, Andreasen and Funk and Dinger for a maximum *
*particle diameter of 32 mm and a minimum particle diameter of 63 μm *

As a result, the range of the fine particles is better represented. Andreasen’s equation was
modified into in Equation 2. They proposed an adjustment factor of *q*= 0.37 for optimum
packing.

min

max min

( )

*q* *q*

*q* *q*

*d* *d*

*P d* *d* *d*

= −

− ^{ (2) }

*d*min minimum particle diameter in the mixture [m]

These curves (Equation 1 and 2) should lead to the mixture with the highest packing density, by combining optimal amounts of differently sized particles. Packing density is defined as the solid volume of particles in a unit volume, or as one minus the porosity.

According to the optimization curves a wider range of the particle size distribution results
in a higher packing density, irrespective of the particle shape. However, particle shape
greatly influences the packing density, especially, when particles of several size classes,
with varying particle characteristics, are used [Walker, 2003; Zheng et al., 1990]. For that
reason, Zheng et al. tried to include particle shape by determining *q* as the average of all

*q*-values for each size class with varying particle shape. Peronius and Sweeting [1985]

presented an equation for calculating the porosity of mixtures, depending on the,

roundness of the particles and the deviation from the Fuller curve. Other researchers, such as [Brouwers and Radix, 2005; Garas and Kurtis, 2008; Hunger, 2010; Kumar and

Santhanam, 2003; Vogt and Lagerblad, 2006] used the model by Funk and Dinger to
optimize their concrete mixtures by adjusting the *q*-value based on their experimental
results or the required workability.

Adjusting mixture composition to a fixed optimization curve is relatively easy since it
requires only a limited amount of input parameters. When the *q* factor is fixed, only the
particle size distributions of the available materials are necessary to optimize a concrete
*mixture. Commercial computer programs such as EMMA [concrete.elkem.com] are *
available. However, particle characteristics like shape or packing density are not taken into
account. The output of the model is an optimized particle size distribution, which not
inevitably leads to a mixture with the highest packing density. This is because optimization
curves are limited with respect to taking into account differences in particle shape and
particle packing of different size groups. Furthermore, Palm and Wolter [2009] and
Stroeven et al. [2003] show that the application of gap graded mixtures can lead to higher
packing densities.

Optimization curves are continuous particle size distributions based on geometrical considerations. Andreasen and Andersen [1930] started with the assumption of a similarity condition that has to be fulfilled as the particles and their environments increase in size. In this way, a change of the size scale should not affect the packing density of the system.

Funk and Dinger [1994] demonstrated that the packing density of continuous particle size distributions (based on this similarity principle) corresponds closely to the packing density of multiple monosized particle groups as described by Furnas [1931]. However, they were not convinced that the packing of discrete (subsection 2.2) and continuous (subsection 2.1) size distributions are actually (mathematically) related [Funk and Dinger, 1994, pp 76]. In 2006 Brouwers demonstrated that the theories on discrete and continuous packings are related mathematically and are actually complementary for packings consisting of multiple particle groups with the same monosized packing density [Brouwers, 2006].

**2.2 Particle packing models **

The purpose of analytical particle packing models is to calculate the theoretical packing density of a mixture. The calculation is based on the particle size distribution and the

packing density of the different particle groups that are present in the mixture.

Mathematical equations are used to determine how particles of different sizes interact geometrically. The two basic mathematical equations of almost all particle packing models are the same and purely based on the geometry of the particles, Equations 3 and 4.

1 1

2 1

*t* 1

*r* *r*

α α

α = =

− large particles (1) are dominant (3)

### ( )

1 2 2

1

*t* *r* *r*

α = + α small particles (2) are dominant (4)

α*t*^{ } calculated packing density of a mixture [-]

α1 packing density of the large size class 1 [-]

α2 packing density of the small size class 2 [-]

*r*1 volume fraction of size class 1 [-]

*r*2 volume fraction of size class 2 [-]. For two size classes, by
definition *r*_{1}+ =*r*_{2} 1

The equations prescribing the packing density were first introduced by Furnas [1929]. They are valid for two monosized groups of particles without interaction between the particles.

Either the amount of large particles is dominating the particle structure and small particles fit in their voids, or the amount of small particles is dominating and large particles are embedded in a matrix of small particles.

Since the equations depend on the particle packing and amount of particles of the monosized groups, they are valid for any type of particle and automatically include particle characteristics such as shape and texture, as long as the particles preserve their shape during packing.

In 1930, Westman and Hugill developed an algorithm that used discrete theory of packing, which could already be used for multiple particle groups without interaction [Westman and Hugill, 1930]. They acknowledged the existence of geometrical particle interaction, but the model did not yet take into account this interaction between particle groups.

In 1931 Furnas published a method to calculate maximum packing density of multiple particle groups as well as an equation to describe the effect of geometrical interaction between two different size classes on the maximum packing density [Furnas, 1931].

Ben Aïm and Le Goff [1967] implemented this effect of geometrical interaction into the Furnas model, by taking into account the influence of the presence large particles on the packing density of small particles (wall effect). In that same period, Schwanda [1966]

published a model which already incorporates both interaction of large particles on small particles (wall effect) and interaction of small particles on large particles (loosening effect) [Reschke, 2000].

The next step in improving particle packing models was the extension from two particle groups to multiple particle groups. Toufar et al. [1976], Stovall et al. [1986] and Yu and Standish [1987] combined the basic equations from Furnas, while Dewar [1999] came up with a stepwise approach where smaller particles are packed in the voids of larger particles and so on.

Nowadays, analytical particle packing models can calculate the packing density of an
entire concrete mixture based on the particle size distributions and packing density of the
materials used in that mixture . The input parameters are the packing density and particle
size distribution of the particle groups, possibly combined with the compaction energy at
which the packing density is measured. The output of an analytical packing model is the
theoretical packing density of the mixture. For mixture optimization, the packing density
of several mixture compositions has to be determined until the maximum packing density
is found. Several models are available for this, but each of them differs in how particle
interaction such as wall effect, loosening effect and/or compaction energy is implemented
in the mathematical equations of the models. Since explaining the differences between the
mathematical equations of these models is not in the scope of this paper, reference is made
to overviews by [Fennis, 2011; Funk and Dinger, 1994; Goltermann et al., 1997; Johansen
and Andersen, 1991; Kumar and Santhanam, 2003]. For readers further interested in using
one of the currently available models, reference is made to Europack [Idorn, 1995; Toufar
*et al., 1976], MixSim [Dewar, 1999; Jones et al., 2002; mixsim.net], 4C-Packing [dti.dk; *

*Glavind et al., 1999], Compressible Packing Model [Larrard, 1999; RENE LCPC or *
*BETONLABPRO via lcpc.fr], the Schwanda model [Geisenhanslucke, 2008; Reschke, 2000; *

Schwanda, 1966], Linear-Mixture Packing Model [Yu and Standish, 1987; 1996] and the Compaction-Interaction Packing Model [Fennis, 2011].

**2.3 Discrete element models **

Discrete element models generate a ‘virtual’ particle structure from a given particle size distribution. In the earliest models, once a particle was placed, its position would not

change anymore. In these static simulations usually particles are randomly positioned in a defined space, starting with the largest particles. The result is a three dimensional space filled with particles of different sizes, which usually do not have contact with each other.

Because of this, the result is officially not a packing or packing structure. Examples of models using static simulations are the hymostruc model [citg.tudelft.nl] or the model used by Zheng and Stroeven [1999] with which e.g. the distribution shown in Figure 2, left hand side, was generated.

*Figure 2: Discrete element models creating a particle structure without particles touching each other *
*(left hand side [Zheng and Stroeven, 1999]) or a stable particle structure (right hand side [Fu and *
*Dekelbab, 2003]) *

With increasing computational speed, the models evolved to dynamic models in which all particles can move. Particles are generated and subsequently move because of forces acting on the particles. For instance, particles can experience gravity and can collide or remain situated. In this way, the resulting packing corresponds to a random loose packing. A disadvantage of this simulation type is, that the resulting packing structure does not have the highest possible packing density that can be achieved with the given particle size distribution [Fu and Dekelbab, 2003]. To solve this, some models generate particles in a container followed by a stepwise decrease of the container volume [Stroeven and Stroeven, 1999]. Other models allow particles to overlap initially and then rearrange the particles while enlarging the container size until no particles overlap [Kolonko et al., 2008].

The result of each simulation is a virtual particle structure in which the size, the shape and the location of all particles are known, see also Figure 2 right hand side. In this way, the virtual structure can be used to assess random particle packing. Packing density can be

calculated from the total occupied volume in the container; however, the particle structure contains much more information. It can be used to evaluate for instance the resistance to external loads [Snoeijer et al., 2003] or the number of contacts between particles. Also it is possible to simulate flowing concrete such as in a slump flow measurement [Gram and Silfwerbrand, 2007; Roussel et al., 2007].

To find the mixture composition with the highest packing density, several mixture compositions should be simulated, which is very time consuming. Especially with broader particle size distributions, computational time increases with hours, because of the high amount of small particles in the mixture. Some researchers like [Kolonko et al., 2008] solve this problem by making use of a stepwise approach in which small particles are packed and then serve as a matrix between larger particles. However, this leads to an increase of input parameters, which already consist of particle size distribution, container size and/or the amount of particles, but should now include several model parameters such as gravity, density, damping, elasticity, shear, friction and particle contact.

For additional information on discrete element modeling and applications, the authors
*refer to other papers in this issue of Heron. *

*2.4 * **Concluding remarks **

The ideal particle size distribution depends on the particle characteristics and therefore it varies with each type of concrete. For instance, when rounded sand is combined with coarse recycled aggregates, the optimal particle size distribution will differ from one of a mixture with angular sand and rounded coarse aggregates. Therefore, one single ideal optimization curve does not inevitably lead to the mixture with the highest packing density. In concrete mixture design high packing density is important to reduce the water content, especially for ultra-high performance concrete and ecological concrete. Analytical particle packing models and discrete element models can calculate the maximum packing density of concrete mixtures. However, due to limitations in computational speed discrete element models are not ideal for concrete mixture optimization, since numerous mixtures have to be evaluated to find the optimal composition. Consequently, at this moment analytical particle packing models provide the best solution for concrete mixture optimization based on particle packing density.

**3 ** **Particle packing and its influence on concrete properties **

Optimizing the particle packing density of concrete mixtures has several advantages for concrete properties in the wet as well as in the hardened state. Adding fine particles to a particle structure helps filling up the voids in the particle structure leaving only minimum space for water. In this way adding fine particles will reduce the water requirement [Kronlöf, 1997; Larrard, 1999; Wong and Kwan, 2008]. Increased packing density of the aggregates, improves strength as long as all voids between the aggregates are filled with cement matrix [Reschke, 2000]. A strong aggregate structure with a high packing density will restrain the amount of shrinkage and creep that can actually be realized. Furthermore, a lower water/cement ratio reduces shrinkage, because of the reduced amount of

evaporable water in the cement paste [Neville, 1995]. Similarly, Kwan and Mora [2001]

reason that a higher packing density leads to a smaller void ratio and thus a smaller amount of cement paste is needed. The heat of hydration and the drying shrinkage are reduced, since both are roughly proportional to the volume of cement paste in the concrete [Kwan and Mora, 2001]. Dhir et al. [2005] demonstrated that changes in the performance of other engineering properties when using particle packing techniques, different cement types and lower water and cement contents, are proportional to the changes in cube compressive strength.

In this section, the advantage of high particle packing density on concrete properties is explained based on the underlying physical relationships. Subsections 3.1 and 3.2 present how particle packing density and particle structure are related to water demand and strength. In subsection 3.3 it is shown how these relations can be used in concrete mixture design.

**3.1 Particle packing density and water demand **

The particle packing density of a concrete mixture has an important influence on its water
demand. The definition of particle packing density α*t* is the solid volume of particles in a
unit volume. However, distinction should be made between the packing density of a stable
particle structure and the volume of particles in a real concrete mixture. In a stable particle
structure all particles are in contact with each other and packed with certain packing
density α*t*. In a real concrete mixture, the partial volume of all the particles in a unit
volume, φ*mix* , is lower. This is shown in Figure 3, where the same amount of particles in a
stable particle structure is packed closer (Fig. 3, middle) than in a real mixture (Fig. 3, left).

In a real concrete mixture part of the water is used to fill the voids between the particles,

while the rest of the water is regarded as excess water. This excess water provides the
flowability of the mixture. Flowability increases with a higher excess of water in the
mixture. In that case, the solid content of the mixture φ*mix** decreases. *

Mixture Stable parcle structure Components

Excess water V^{ew}
Void water V^{vw}

Parcles V^{p}

*Figure 3: The volume of a flowable mixture compared to the volume occupied by a stable particle *
*structure containing the same particles *

If the particle composition of a concrete mixture is optimized in such a way that the maximum particle packing density increases, less void water is necessary. Because of this effect high packing density improves the workability of a mixture. When part of the water that first filled up the voids between the particles, becomes available as excess water, it will provide more flowability. Clearly, the resulting increase in flowability is very useful in the design of concrete mixtures.

In Figure 4 the relation between flow value and packing density for more than 60 tested
mortar mixtures is shown [Fennis, 2011]. The results are presented as a function of the ratio
between solid volume in the real mixtures φ*mix* and the maximum calculated packing
density α*t*.

The relation between packing density and water demand can be used to predict the
required amount of water of a mixture. An increased packing density lowers the required
amount of void water. Therefore, concrete mixtures with the same workability can be
designed with a lower water requirement. In this way, increasing the packing density
enables the design of high strength concrete with low water/cement ratio or ecological
*concrete with a constant water/cement ratio but a lower amount of cement. *

R² = 0.87

0 50 100 150 200 250

0.85 0.9 0.95 1

Flow value [mm]

φ_{mix}/α_{t}[m^{3}]
Mortar mixtures

* Figure 4: The flow value as a function of φ**mix**/α**t** for mortar mixtures [Fennis, 2011] *

**3.2 Packing density and cement spacing **

Optimizing the packing density is not only beneficial for the water demand, but it can also decrease the space between the cement particles. This space between the cement particles depends on the amount of water in a mixture as well as the particle structure of the mixture. With a high packing density in the mixture, cement particles and other particles are close to each other, reducing the space that needs to be filled by hydration products.

This leads to high strengths. The other way around, with higher amounts of water and higher water/cement ratios, the cement particles are further apart. Therefore, during the hydration process, the hydration products of the cement particles need to bridge a larger distance, eventually leading to lower strengths.

Traditionally, water/ cement ratio (or a derived parameter) is the basis of most

equations for predicting the strength of concrete [Abrams, 1919; Bolomey, 1935; Féret, 1897;

Larrard, 1999; Mechling et al., 2007; Mikulić et al., 2008; Neville, 1995; Popovics, 1998;

Powers, 1968; Souwerbren, 1998]. However, by using particle packing technology the cement spacing can be better predicted than by using water/cement ratio and volume fractions alone. By making use of the entire particle structure as prescribed by a discrete element model or in this case an analytical particle packing model, it is possible to calculate the space available for cement particles for strength predictions or even hydration

simulations. Incorporating the entire particle structure by using particle packing models provides more advanced information for mixture design, because also the size of fillers and aggregates can be taken into account.

The space between the cement particles can be described by the Cement Spacing Factor
*CSF (Equation 5). This Cement Spacing Factor consists of two parts: the space between the *
particles in a stable particle structure and a volume factor to account for the water in the
mixture.

*cem* *cem* *mix*

*t* *cem* *t*

*cem*
*mix*

*CSF* _{∗}

∗

ϕ ϕ ϕ

= ϕ α =ϕ α

ϕ

(5)

*CSF* cement spacing factor [-]

ϕ*cem* partial volume occupied by the cement in a stable particle structure [-]

**cem*

ϕ maximum partial volume that the cement may occupy given the presence of other particles [-]

ϕ*mix* partial volume of all the particles in a mixture in a unit volume [-]

α*t* calculated packing density of a mixture [-]

As a measure of the space between the cement particles in a stable particle structure, the
*value φ**cem**/φ***cem** is used. In this relation φ**cem* is the volume in the mixture which is occupied
*by the cement. φ***cem* is the maximum volume that cement may occupy given the presence of
*the other particles. As such, φ**cem**/φ***cem* represents the free space surrounding the cement
*particles on a volume basis. In principle, more cement particles in a mixture (higher φ**cem*)
will lead to a closer cement spacing. Addition of fine fillers creates higher packing density
*(leading to a smaller φ***cem*) and thus closer cement spacing.

In a real mixture, not only the voids in the stable particle structure are filled with water,
but some excess water is always present to allow flowability, see Figure 3. A stable particle
structure is defined as a structure of particles in which all particles are in contact with one
or more particles in such a way that the packing structure is stable under the influence of
*gravity. By adding the water, all particles move away from each other by the factor α**t**/φ**mix*.
Therefore adding more water leads to larger distances between the cement particles and
thus to lower strength.

Figure 5 shows the relation of Cement Spacing Factor to the compressive strength of 48 mortar mixtures [Fennis, 2011]. In Figure 6, an example is presented of how particle packing density of mixtures can influence the spacing between the cement particles. When cement is replaced by coarse fillers, with a similar size as cement, the spacing between the cement particles increases. This can be explained by considering a container filled by cement particles. If 20% of the cement is replaced by a filler of similar size, the packing

density remains constant. In total the same volume percentage of the container is still occupied by the particles, however, now only 80% of the original cement particles are present in that container. Thus the cement particles are relatively further away from each other (Figure 6 left hand side). However, when cement is replaced by finer particles (for instance M600, see also Section 4) the packing density increases. In that case, the 80%

cement particles will fit in a smaller container (Figure 6, right hand side) and therefore the space between the cement particles is smaller than with the coarse filler [Fennis, 2012].

R^{2} = 0.91

0 10 20 30 40 50 60 70

0.68 0.7 0.72 0.74 0.76 0.78 0.8 0.82

CSF [-]

Strength [N/mm2 ]

E1-E9, without M600 Series F

Series H

E10-E13, with M600

*Figure 5: Cube compressive strength of mortars in relation to Cement Spacing Factor CSF [Fennis, *
*2011] *

* *

F

F

C

C C

C

C C

*Figure 6: The volume occupied by a stable particle structure with coarse filler (F) compared to the *
*volume occupied by a stable particle structure with fine filler (C=Cement) *

**3.3 Cyclic design procedure for ecological concrete **

The relations between packing density and water demand, and between particle structure and cement spacing can be used in the design of concrete mixtures. To use these relations in concrete mixture design for ecological concrete, a three step cyclic design procedure has been developed as presented in Figure 7. The design procedure usually starts by

calculating the packing density of a new mixture (top corner), but can also start with a mixture adjustment of a reference mixture (bottom, right corner).

### strength water

### packing

φ^{m}

ix

### /

^{α}

^{t}

CSF

Mixtu re a

djustm ent

### strength water

### packing

φ^{m}

ix

### /

^{α}

^{t}

CSF

Mixtu re a

djustm ent

*Figure 7: Cyclic design procedure for ecological concrete *

For the particle packing optimization (top corner) it is convenient to start from an existing mixture and use an analytical particle packing model such as the compaction-interaction packing model [Fennis, 2011] to find a mixture composition with a higher packing density.

Also mixture optimization based on other models (Section 2) could be used as long as the model provides a good calculation of the particle packing density of all the solid

constituents in the mixture. The output of the particle packing model in this step will be a
*mixture composition with its corresponding packing density α**t*.

* In the next step the water demand of the mixture is determined by using φ**mix**/α**t*, see
*Subsection 3.1. This value is directly related to the flowability of a mixture, so φ**mix* and thus
the volume of water can be adjusted to the required consistency. When water absorption of
the materials and predicted air content are available, the amount of water to be dosed
during the mixing process can be adjusted here.

In the following step the strength is predicted on the basis of this mixture composition, its packing density and its particle structure. The strength prediction is based on the

assumption that in low strength ecological concrete all aggregates are stronger than the produced concrete. In that case, the cement glues the aggregates together and the strength depends on the spacings to be bridged to connect all aggregates. With a high packing density in the mixture, cement particles and other particles are close to each other, reducing the space that needs to be filled by hydration products, which leads to higher strengths. With higher amounts of water and higher water/cement ratios, the cement particles are further apart, eventually leading to lower strengths. With this concept, expressed by the Cement Spacing Factor (CSF), the strength of a mixture can be predicted [Fennis, 2011].

In the last step of the cycle, the requirements of the user are taken into account to adjust the mixture composition. In the research project presented in this paper, the requirement is the strength of the concrete. If the predicted strength in the last step is higher than the desired strength, the cement content can be lowered in the next step. Furthermore, additional user defined requirements can be used such as a minimum amount of powders or a fixed proportion of cement to powders. Since the mixture composition is adjusted to the requirements in this step, the particle size distribution might change again.

Cyclic design is necessary as long as one of the material fractions change in the last design step. For instance, when the cement content is lowered due to a high predicted strength value, this changes the overall particle size distribution and thus the packing density. In that case the cyclic design procedure is repeated until the mixture composition does not change anymore in the last design step.

**4 ** **Experimental program ecological concrete **

As a demonstration, the design method prescribed in Subsection 3.3 is used to design three
ecological concrete mixtures. The mixtures were designed for strength class C20/25 with
minimum amounts of cement CEM I 42.5 N (ENCI). Three types of cement replacing
materials were used: fly ash because of its ball bearing effect and high packing density,
quartz powder because of its fine and narrow particle size distribution, and ground
incinerator bottom ash as residual product with low environmental impact. The materials
used in the mixtures were: Portland cement CEM I 42.5 N (ENCI Maastricht), blast furnace
slag cement CEM III/B 42.5 N (ENCI IJmuiden), Fly ash (Vliegasunie), bottom ash
*(INASHCO), quartz powder M600: d*50=3 μm (Sibelco), river sand and coarse aggregates
(Filcom, Papendrecht) and Glenium 51 con 35 (BASF).

The mixture compositions of the three ecological mixtures and their reference mixture are
presented in Table 1 as series A. The particle size distributions of the mixtures are
presented in Figure 8. The reference mixture A1 was designed with 260 kg cement per m^{3}
concrete, which is the minimum cement content according to the Dutch standards. Since
the mixture was designed for strength class C20/25 with design strength 33 N/mm^{2}, a
relatively high amount of water had to be dosed. Mixture A2 and A3 were optimized on
packing density. Using the design cycle as presented in Section 2 the cement content was
minimized to 110 kg/m^{3}, in order to reach the estimated design strength of 33 N/mm^{2}.
Mixture A2 contained a combination of fly ash and quartz powder M600. In mixture A3
also blast furnace slag cement was used to increase the packing density even further and
create a more ecological mixture containing less Portland clinker. Mixture A4 was
designed with wet ground municipal solid waste incinerator bottom ash from INASHCO.

*Figure 8: Particle size distribtuions of concrete mixtures series A combined with workability *
*recommendations of [NEN-EN 5950: 1995 nl] and Dinger and Funk optimization curve for q =0.37 *

To determine the strength development in time, cube compressive strength and tensile splitting strength were measured according to [NEN-EN 12390:2009] on 150 mm cubes after 2, 7, 28, 56 and 90 days. At every point in time three specimens for compressive strength and three specimens for splitting tensile strength were tested. Furthermore, prism compressive strength and modulus of elasticity were determined after 28 days. The experiment was executed by loading three 100×100×400 mm prisms with a constant

deformation speed of 10^{-3} mm/s. The longitudinal displacements were recorded
continuously by means of four LVDT’s per specimen, which were placed in longitudinal
direction in the center of the long sides with 136 mm measuring length.

Drying shrinkage and creep of the ecological mixtures were measured on six 100×100×400 mm concrete prisms in the longitudinal direction over a distance of 200 mm. Shrinkage testing started after 7 days of hardening at 20⁰C, 95% RH. Creep measurement started after 28 days of hardening, of which 7 days at 20⁰C, 95% RH and 21 days at 20⁰C, 50% RH. For the creep measurement a force of 0.33 times the prism compressive strength was applied.

The prism compressive strength was determined on specimens of the same size, which hardened under the same conditions as the creep specimens. All shrinkage and creep tests were conducted for 90 days at 20⁰C and 50% RH.

The electrical resistance is measured at a frequency of 120 Hz on a saturated 150×150×150 mm concrete cube tightened between two steel plates. Measurements were taken on surface dried, saturated cubes at 20 ± 2⁰C and 65 ± 5% relative humidity. Other durability aspects such as chloride penetration and microstructural development were evaluated in a parallel research project on low cement content concrete and will be presented in [Valcke et al., 2013].

**5 ** **Experimental results ecological concrete **

Evaluation of the fresh state of the ecological concrete mixtures showed that all mixtures in series A were homogeneous and stable. Results for slump [NEN-EN 12350-2:2009], air content [NEN-EN 12350-7:2009] and density [NEN-EN 12350-6:2009] are presented in Table 1. All the mixtures had sufficient workability for casting and vibration. Mixture A3 was judged as harsh compared to the other mixtures, which was especially noted when filling the moulds. To increase the ability to cast in practice, it is recommended to increase the total powder content. This will also improve the cohesion of the mixtures which was evaluated as low for mixtures A3 and A4, leading to easy collapse of the slump. These two mixtures had similar workability as mixture A2, consistency class C1 earth moist. Very low segregation and little bleeding of the mixtures was observed, by virtue of the dense particle structure.

*Table 1: Mixture compositions [kg/m*^{3}*] and the measured material properties of series A *

** Mixtures **

**Composition ** **A1 A2 A3 A4 **

CEM I 42.5 N [kg/m^{3}] 260 110 44 125

CEM III/B 42.5 [kg/m^{3}] - - 66 -

Fly ash SMZ Maasvlakte [kg/m^{3}] - 88 65 75

Quartz powder M600 [kg/m^{3}] - 62 85 -

Ground IBA [kg/m^{3}] - - - 50

Aggregates 4-16 [kg/m^{3}] 1193 1162 1160 1157

Sand 0-4 [kg/m^{3}] 718 867 866 864

Glenium 51 [% kg/kg of powders] [%] 0.8 0.8 1.2 1.2

Effective amount of water [kg/m^{3}] 162 103 103 112

Water/cement ratio [-] 0.62 0.94 0.94 0.90

Water/powder ratio [-] 0.62 0.40 0.40 0.45

Estimated density (1% air) [kg/m^{3}] 2351 2409 2408 2402

Packing density CIPM [-] 0.886 0.897 0.898 0.890

**Rheological properties **

Slump [cm] 20 3 *12 14 *

Air content [%] 0.9 1.8 0.9 0.9

Density [kg/m^{3}] 2366 2406 2424 2456

**Mechanical properties **

2-day cube compressive strength [N/mm^{2}] 13.9 15.2 7.2 12.9
7-day cube compressive strength [N/mm^{2}] 24.2 25.2 17.6 22.9
28-day cube compressive strength [N/mm^{2}] 32.1 39.6 33.5 37.9
56-day cube compressive strength [N/mm^{2}] 36.4 39.9 35.3 48.0
90-day cube compressive strength [N/mm^{2}] 36.4 53.1 39.1 55.1
7-day tensile splitting strength [N/mm^{2}] 2.0 2.1 1.4 2.0
28-day tensile splitting strength [N/mm^{2}] 2.5 2.7 2.5 3.0
56-day tensile splitting strength [N/mm^{2}] 2.6 2.7 3.0 3.3
90-day tensile splitting strength [N/mm^{2}] 2.7 3.7 2.6 4.0
28-day prism compressive strength [N/mm^{2}] 29.5 26.6 20.0 29.1
28-day modulus of elasticity [N/mm^{2}] 30500 32500 30500 30500

The cube compressive strength development of series A is presented in Table 1. All
mixtures reach the design strength of 33 N/mm^{2} for strength class C20/25 within 28 days.

The contribution of the fly ash and quartz powder to decrease the water demand is substantial. However, neither the conventional water/cement ratio nor the water/binder ratio of mixtures A2 and A3 can explain the strengths attained by these mixtures. Mixture A2 has a water/cement ratio of 0.94 and a water/binder ratio of 0.83 [NEN-EN 206-1:2001].

Mixture A3 has a water/cement ratio of 0.94 and a water/binder ratio of 0.89. Based on the
water/binder ratio the 28-day strength of these mixtures should have been between 20 and
25 N/mm^{2}. The additional strength gain up to 39.6 N/mm^{2} for mixture A2 and up to 33.5
N/mm^{2} for mixture A3 is explained by the high particle packing density of the powders
and possible additional pozzolanic effects of the fly ash and quartz powder both
improving the microstructure of the concrete. This is also confirmed by the electrical
resistance measurements. Mixture A4 contained ground incinerator bottom ash as cement
replacing material and reaches a 28-day cube compressive strength of 37.9 N/mm^{2}.

The relationship between the average cube compressive strength and the tensile splitting strength of the ecological mixtures is the same as for normal concrete. Also the measured moduli of elasticity of the ecological mixtures comply with the relation for compressive strength versus modulus of elasticity as described in Eurocode 2 for normal concrete. Only mixture A4 has a relatively low modulus of elasticity compared to its cube compressive strength. The correspondence of the ecological mixtures to the standard relations proves the possibility to design for cube compressive strength in the cyclic design procedure.

0 0.1 0.2 0.3 0.4 0.5

0 28 56 84

Shrinkage [mm/m]

Time [day]

Ref - A1 A2 A3 A4 Eurocode 2

* * * Figure 9: Shrinkage of mixtures series A compared to Eurocode 2 *

The measured drying shrinkage and creep of the ecological mixtures A2 and A3 were relatively low compared to normal concrete with the same compressive strength. The results can be explained by the relatively low cement content, the normal modulus of elasticity and the high density of the particle structure, which provides resistance against deformation of the cement matrix. In Figures 9 and 10 the shrinkage and creep are compared with corresponding formulations in Eurocode 2 [NEN-EN 1992-1-1:2005] for concrete in strength class C20/25. Mixture A4 has a relatively higher shrinkage than mixtures A2 and A3. In the first 77 days this shrinkage is even larger than the shrinkage of the reference mixture A1. The shrinkage of both reference mixture A1 and mixture A4 is still lower than the shrinkage estimation according to Eurocode 2. The creep of reference mixture A1 is larger than was expected based on its strength class and Eurocode 2.

The variation in the shrinkage and creep measurements of the different mixtures shows that shrinkage and creep very much depend on the types of fillers and binders which are used in the ecological concrete. When for a certain application shrinkage or creep is the most important mixture design criterion, performance-based design will lead to optimal ecological concrete.

0 0.5 1 1.5 2 2.5 3

0 28 56 84

Creep coefficient [-]

Time [day]

Ref - A1 A2 A3A4 Eurocode 2

* Figure 10: Creep of mixtures series A compared to Eurocode 2 *

An indication of the durability of ecological concrete can be provided by measuring the permeability of concrete, since concrete with lower permeability is less sensitive for transport mechanisms such as chloride ingress. The two electrode method (TEM) is used to

determine the electrical resistance of concrete and provides an indirect measurement of the amount of uninterrupted water in a fully saturated specimen. This amount of water is related to the quantity of continuous pores in the concrete and thus also to the permeability of the concrete. From theoretical and experimental work there appears to be a relationship between resistivity of and chloride diffusion in a particular concrete composition [Andrade et al., 1993; Polder, 1995; Polder, 2000]. Furthermore, Smith [2006] reports that electrical resistance measurements are related to chloride penetration resistance as measured by the rapid chloride permeability test.

The resistivity of the three ecological mixtures is higher than the resistivity of reference mixture A1, Figure 11, which is positive to prevent ion ingress. Mixtures containing blast furnace slag cement often show high resistivities, caused by differences in microstructure and pore solution conductivity. This explains the differences in the resistivity of A2 compared to A3. The resistivity was not related to the water/cement ratio or water/binder ratio. In fact, mixture A2 with a water/cement ratio of 0.94 and a water/binder ratio of 0.83 has a much better resistivity than A1 with a water/cement ratio of 0.62.

The electrical resistance measurements show that predicting concrete properties related to durability by using the water/cement ratio, the water/binder ratio and/or the cement content is not reliable. To evaluate the durability, the total composition of the mixture specified by the particle size distribution, water content, cement content and

water/powder ratio, should be taken into account. For durability aspects, extensive research on performance-based design is recommended.

### 0 50 100 150 200 250 300 350 400

### 0 28 56 84

### R esistiv ity [O hm ·m ]

### Time [day]

### A1 A2 A3 A4

* Figure 11: Results of resistivity measurements (TEM) of series A *

**6 ** **Conclusions **

The packing density of a particle mixture by itself is a powerful parameter in the design of concrete mixtures. It helps to determine the suitability of aggregates and fillers for the use in concrete mixtures. In fact, particles should contribute to a higher packing density and to a reduced water demand. Whether adding particles to a concrete mixture indeed has this desired effect, can be determined by particle packing models. In this paper three different methods to determine the particle distribution of a mixture are presented; optimization curves, particle packing models and discrete element modelling.

Higher packing densities leave less space for voids to be filled with water, which reduces the water demand and increases the strength of concrete mixtures. Via the packing structure, the amount of water in a real mixture and the Cement Spacing Factor CSF it is possible to predict the strength of concrete. These relations can be used in a cyclic design procedure to optimize mixture compositions of, for instance, ecological concrete.

Based on experiments on ecological concrete it was demonstrated how particle packing
technology can be effective to lower cement contents, without changing concrete properties
in a negative way. Three ecological concrete mixtures were designed containing fly ash,
quartz powder and ground incinerator bottom ash, thereby saving up to 57% of Portland
cement and reducing the CO2-emission of concrete with 25% [Fennis, 2011]. By making use
of the cyclic design method all ecological mixtures reached at least their predicted design
strength of 33 N/mm^{2}. The mixtures were tested on compressive strength, tensile strength,
modulus of elasticity, shrinkage, creep and electrical resistance. The results confirmed that
relationships between cube compressive strength, tensile splitting strength and modulus of
elasticity correspond to those for normal concrete. Furthermore, the particle packing
optimization resulted in a stiff and strong particle structure, which had a positive influence
on concrete properties such as shrinkage and creep. However, concrete properties such as
shrinkage, creep and electrical resistance can significantly be influenced by the

mineralogical composition of the filler and binders. The electrical resistance tests on these ecological mixtures showed that the increased packing density and reduced water demand eventually lead to a denser microstructure of the concrete. The experimental program showed that it is possible to design ecological concrete in which 50% of the cement is saved by using particle packing technology in concrete mixture optimization.

**Acknowledgements **

This research was supported by the Dutch Technology Foundation STW, applied science division of NWO and the Technology Program of the Ministry of Economic Affairs. The experiments were performed by the technicians of the Stevin Laboratory of Delft University of Technology, which is very much appreciated.

**References **

*Abrams, D.A. (1919) Design of Concrete Mixtures. Bulletin 1, Structural Materials Research *
*Laboratory, Lewis Institute, Chicago *

Andrade, C., Sanjuan, M.A. and Alonso, M.C. (1993) Measurement of chloride diffusion
*coefficient from migration tests. NACE Corrosion '93, paper 319 *

Andreasen, A.H.M. and Andersen, J. (1930) Über die Beziehung zwischen Kornabstufung und Zwischenraum in Produkten aus losen Körnern (mit einigen Experimenten).

*Colloid & Polymer Science, Vol. 50 (3), pp. 217-228. *

Ben Aïm, R. and Le Goff, P. (1967) Effet de paroi dans les empilements désordonnés de
*spheères et application à la porosité de mélanges binaires. Powder Technology, Vol. 1 *
(5), pp. 281-290.

*Bolomey, J. (1935) Granulation et prevision de la résistance probable des bétons. Travaux *
19(30): 228-232

Brouwers, H.J.H. and Radix, H.J. (2005) Self-Compacting Concrete: Theoretical and
*experimental study. Cement and Concrete Research, Vol. 35, pp. 2116-2136. *

Brouwers, H.J.H. (2006) Particle-size distribution and packing fraction of geometric
*random packings. Physical Review E - Statistical, Nonlinear, and Soft Matter Physics. Vol. *

74 (3), pp. 031309- 031309-14.

*Dewar, J.D. (1999) Computer Modelling of Concrete Mixtures. London: E & FN Spon. *

Dhir, R.K., McCarthy, M.J. and Paine, K.A. (2005) Engineering property and structural
*design relationships for new and developing concretes. Materials and Structures, Vol. 38 *
(275), pp. 1-9.

Fennis S.A.A.M., Walraven J.C., Uijl J.A. den (2013) Compaction-interaction packing model: an extended basis to design concrete mixtures including aggregates and fillers.

*Materials and Structures, Vol. 46, pp. 463-478,479 DOI 10.1617/s11527-012-9910-6; DOI *
10.1617/s11527-013-0014-8

*Fennis S.A.A.M. (2011) Design of Ecological Concrete by Particle Packing Optimization, PhD *
Thesis, Delft: Delft University of Technology, http://repository.tudelft.nl/assets/

uuid:5a1e445b-36a7-4f27-a89a-d48372d2a45c/fennis_final.pdf

*Féret, R. (1892) Sur la compacité des mortiers hydrauliques. Annales des Ponts et Chaussees. *

Vol. 4 (2e semestre), pp. 5-16.

*Féret, R. (1897) Etudes sur la constitution intime des mortiers hydrauliques. Bulletin de la *
*Socit d'Encouragement pour l'Industrie Nationale 2, pp. 1591-1625. *

Fu, G. and Dekelbab, W. (2003) 3-D random packing of polydisperse particles and concrete
*aggregate grading. Powder Technology, Vol. 133, pp. 147-155. *

*Fuller, W.B. and Thompson, S.E. (1907) The laws of proportioning concrete. ASCE J. *

*Transport., Vol. 59, pp. 67-143. *

*Funk, J.E. and Dinger, D.R. (1994) Predictive Process Control of Crowded Particulate *
*Suspensions - Applied to Ceramic Manufacturing. Boston: Kluwer Academic Publishers. *

Funk, J.E., Dinger, D.R. and Funk, J.E.J. (1980) Coal Grinding and Particle Size Distribution Studies for Coal-Water Slurries at High Solids Content. Final Report, Empire State Electric Energy Research Corporation (ESEERCO). New York.

*Furnas, C.C. (1929) Flow of gasses through beds of broken solids. Bureau of Mines Bulletin *
307.

Furnas, C.C. (1931) Grading Aggregates; Mathematical Relations for Beds of Broken Solids
*of Maximum Density. Industrial and Engineering Chemistry. Vol. 23 (9), pp. 1052-1058. *

Garas, V.Y. and Kurtis, K.E. (2008) Assessment of methods for optimising ternary blended
*concrete containing metakaolin. Magazine of Concrete Research, Vol. 60 (7), pp. 499-510. *

*Geisenhanslüke, C. (2008) Einfluss der Granulometrie von Feinstoffen auf die Rheologie von *
*Feinstoffleimen. Fachbereich Bauingenieurwesen. PhD Thesis. Kassel: Universität Kassel. *

Glavind, M., Olsen, G.S. and Munch-Petersen, C. (1999) Packing Calculations and concrete mix design. Danish Technological Institute.

Goltermann, P., Johansen, V. and Palbøl, L. (1997) Packing of Aggregates: An Alternative
*Tool to Determine the Optimal Aggregate Mix. ACI Materials Journal, Vol. 94 (5), pp. *

435-443.

Gorkum, C.O.M. van (2010) CO2 emissions and energy consumption during the construction of concrete structures: Comparison between prefab and insitu concrete viaducts. Master thesis Delft University of Technology.

*Gram, A. and Silfwerbrand, J. (2007) Computer simulation of SCC flow. Betonwerk und *
*Fertigteil-Technik/Concrete Plant and Precast Technology, Vol. 73 (8), pp. 40-48. *

*Hunger, M. (2010) An integral Design Concept for Ecological Self-Compacting Concrete. *

Bouwkunde. PhD Thesis. Eindhoven: Eindhoven University of Technology.

Idorn, G.M. (1995) Europack V1.1 User Manual Europack (G.M. Idorn Consult A/S, Denmark).

Johansen, V. and Andersen, P.J. (1991) Particle Packing and Concrete Properties. In:

*Skalny, J. and Mindess, S. (eds). Materials science of concrete 2. Westerville: American *
Ceramic Society.

Jones, M.R., Zheng, L. and Newland, M.D. (2002) Comparison of particle packing models
*for proportioning concrete constituents for minimum voids ratio. Materials and *
*structures, Vol. 35, pp. 301-309. *

Kolonko, M., Raschdorf, S. and Wäsch, D. (2008) A Hierarchical Approach to Estimate the Space Filling of Particle Mixtures with Broad Size Distributions. pp. 28.

*Kronlöf, A. (1997) Filler effect of inert mineral powder in concrete. VTT Technical research *
centre of Finland. Espoo, Finland.

Kumar, S.V. and Santhanam, M. (2003) Particle packing theories and their application in
*concrete mixture proportioning: A review. The Indian Concrete Journal, Vol. 77 (9), pp. *

1324-1331.

Kwan, A.K.H. and Mora, C.F. (2001) Effects of various shape parameters on packing of
*aggregate particles. Magazine of Concrete Research, Vol. 53 (2), pp. 91-100. *

*Larrard, F. de (1999) Concrete mixture proportioning: a scientific approach. London: E & FN *
Spon.

Mechling, J., Lecomte, A. and Diliberto, C. (2007) The influence of the clinker composition
*on concrete compressive strength. Concrete under Severe Conditions: Environment & *

*Loading CONSEC 2007. Tours, France. *

*Mehta, P.K. (2001) Reducing the environmental impact of concrete. Concrete International, *
October 2001, pp. 61-66.

Mikulić, D., Gabrijel, I. and Milovanović, B. (2008) Prediction of concrete compressive
*strength. International RILEM Symposium on Concrete Modelling - CONMOD'08. Delft, *
the Netherlands.

*Neville, A.M. (1995) Properties of Concrete. Harlow: Longman. *

Palm, S. and Wolter, A. (2009) Determining and optimizing the void filling of dry particle
*systems. Cement International, Vol. 7 (1/2009), pp. 1-8. *

Peronius, N. and Sweeting, T.J. (1985) On the correlation of minimum porosity with
*particle size distribution. Powder Technology, Vol. 42 pp. 113-121. *

Polder, R.B. (1995) Chloride diffusion and resistivity testing of five concrete mixes for
*marine environment, In Nilsson, L.-O. and Ollivier, P. (eds). Proc. RILEM. International *
*Workshop on Chloride Penetration into Concrete, St-Remy-les-Chevreuses, France, pp 225-*
233.

Polder, R. B. (2000) Test methods for on site measurement of resistivity of concrete (Draft
*Technical Recommendation RILEM TC 154-EMC). Materials and Structures, Vol. 33, pp. *

603-611

Popovics, S. (1998) History of mathematical model for strength development of Portland
*cement concrete. ACI Materials Journal, Vol. 95 (5), pp. 593-600. *

*Powers, T.C. (1968) The Properties of Fresh Concrete. New York: Wiley. *

*Reschke, T. (2000) Der Einfluss der Granulometrie der Feinstoffe auf die gefügeentwicklung und *
*die Festigkeit von Beton. VBT Verlag Bau+Technik GmbH. Düsseldorf. *

Roussel, N., Geiker, M.R., Dufour, F., L.N., T. and Szabo, P. (2007) Computational
*modelling of concrete flow: General overview. Cement and Concrete Research, Vol. 37, *
pp. 1298-1307.

Schwanda, F. (1966) Das rechnerische Verfahren zur Bestimmung des Hohlraumes und Zementleimanspruches von Zuschlägen und seine Bedeutung für Spannbetonbau.

*Zement und Beton, Vol. 37, pp. 8-17. *

*Smith, D. (2006) The Development of a Rapid Test for Determining the Transport Properties of *
*Concrete. Master thesis: University of New Brunswick *

Snoeijer, J.H., Hecke, M.v., Somfai, E. and Saarloos, W.v. (2003) Packing geometry and
*statistics of force networks in granular media. Physical Review E - Statistical, Nonlinear, *
*and Soft Matter Physics, Vol. 70 (1 1), pp. 15. *

*Souwerbren, C. (1998) Betontechnologie. Stichting Betonprisma.-III, tiende druk, ‘s-*
Hertogenbosch.

Stovall, T., Larrard, F. de and Buil, M. (1986) Lineair Packing Density Model of Grain
*Mixtures. Powder Technology, Vol. 48, pp. 1-12. *

Stroeven, P. and Stroeven, M. (1999) Assessment of packing characteristics by computer
*simulation. Cement and Concrete Research, Vol. 29, pp. 1201-1206. *

Stroeven, P., Stroeven, M. and Bui, D.D. (2003) On optimum packing density. In: Shu Yuan,
*Y., Shah, S.P. and Lin Lü, H. (eds). Proceedings of International Conference on Advances in *
*Concrete and Structures, Rilem Publications SARL, pp. 793-800. *

Talbot, A.N. and Richart, F.E. (1923) The strength of concrete in relation to the cement,
*aggregates and water. University of Illinois Engineering Experiment Station, Bulletin No. *

137.

Toufar, W., Born, M. and Klose, E. (1976) Beitrag zur Optimierung der Packungsdichte Polydisperser körniger Systeme. Freiberger Forschungsheft A 558, VEB Deutscher Verlag für Grundstoffindustrie, pp. 29-44.

Valcke, S.L.A., Polder, R.B., Nijland, T.G., Leegwater, G.A., Visser, J.H.M. and Bigaj-van
Vliet, A.J. (2013) High filler concrete using fly ash - Chloride penetration and
*microstructure, HERON 57 (2012), No. 3, pp. 169-184. *

Vogt, C. and Lagerblad, B. (2006) Ultrafine particles to save cement and improve concrete
*properties. Advances in cement and concrete X. July 2-7, Davos, Switzerland. *

Walker, W.J. (2003) Persistence of Granular Structure during Compaction Processes.

*KONA, Vol. 21, pp. 133-142. *

*Westman, A.E.R. and Hugill, H.R. (1930) The packing of particles. Journal of the American *
*Ceramic Society, Vol. 13 (10), pp. 767-779. *

Wong, H.H.C. and Kwan, A.K.H. (2008) Packing density of cementitious materials:

*measurement and modelling. Magazine of Concrete Research, Vol. 60 (3), pp. 165-175. *

Yu, A.B. and Standish, N. (1987) Porosity calculations of multi-component mixtures of
*spherical particles. Powder Technology, Vol. 52, pp. 233-241. *

Yu, A.B., Zou, R.P. and Standish, N. (1996) Modifying the Linear Packing Model for
*Predicting the Porosity of Nonspherical Particle Mixtures. Ind. Eng. Chem. Res., Vol. 35 *
pp. 3730-3741.

Zheng, J., Johnson, P.F. and Reed, J.S. (1990) Improved Equation of the Continuous Particle
*Size Distribution for Dense Packing. Journal of the American Ceramic Society, Vol. 73 (5), *
pp. 1392-1398.

Zheng, J. and Stroeven, P. (1999) Computer-simulation of particle section patterns from
*sieve curve for spherical aggregate. In: Dhir, R.K. and Dyer, T.D. (eds). Modern concrete *
*materials: binders, additions and admixtures: proceedings of the international Conference held *
*at the University of Dundee, Scotland, UK on 8-10 September. *

**Standards **

NEN-EN 206-1:2001. Concrete - Part 1:Specification, performance, production and conformity.

NEN-EN 1992-1-1:2005. Eurocode 2: Design of concrete structures - Part 1-1: General rules and rules for buildings.

NEN-EN 12350-2:2009. Testing fresh concrete - Part 2: Slump-test.

NEN-EN 12350-6:2009. Testing fresh concrete - Part 6: Density.

NEN-EN 12350-7:2009. Testing fresh concrete - Part 7: Air content - Pressure methods.

NEN 5950:1995 nl. Voorschriften Beton Technologie (VBT 1995). Eisen, vervaardiging en keuring. Withdrawn.

**Websites **

www.citg.tudelft.nl/index.php?id=17650&L=1 Hymostruc free download.

www.elkem.com/en/Silicon-materials/Support/Software-EMMA/ Software EMMA.

www.dti.dk/2783 4C-Packing ecosmartconcrete.com

www.lcpc.fr/francais/produits/lcpc-produits-betonlabpro/ RENÉ-LCPC minerals.usgs.gov/minerals/pubs/commodity/cement/mcs-2012-cemen.pdf www.mixsim.net/ Software MixSim

www.pbl.nl/en/publications/2011/long-term-trend-in-global-co2-emissions-2011-report